Mechanical Properties of graphene. Gyan Prakash. Department of Physics, and The Birck Nanotechnology Center, Purdue University. March 23,2009. Class-Presentation Phys-570X. Science, 315 , 2007. Demonstrate how single and multilayer graphene sheets can be mechanically actuated.
Department of Physics, and
The Birck Nanotechnology Center,
Fig. 1. (A) Schematic of a suspended graphene resonator. (B) An optical image of a double –layer graphene sheet that becomes a single suspended layer over the trench. Scale bar, 2 mm. Each colored circle corresponds to a point where a Raman spectrum was measured. (C) Raman signal from a scan on the graphene piece. Each colored scan is data taken at each of the matching colored circles. The top scan is used as a reference and corresponds to the Raman shift of bulk graphite. (D) An optical image of few-layer (~4) graphene suspended over a trench and contacting a gold electrode. Scale bar, 1 mm. (Inset) A line scan from tapping mode AFM corresponding to the dashed line in the optical image. It shows a step height of 1.5 nm. (E) A scanning electron microscope image of a few-layer (~2) graphene resonator. Scale bar, 1 mm.
Raman Scattering from High-Frequency Phonons in Supported n-Graphene Layer Films : A. Gupta, G. Chen et al. Nano Lett., 2006, 6 (12), 2667-2673• DOI: 10.1021/nl061420a
Effective nGL film height vs assigned n. The straight line is a least-square fit to the data. The apparent thickness of a graphene layer is t ) 0.35 ( 0.01 nm, and the AFM offset parameter is t0 ) 0.33 nm
High-frequency first- and second-order microRaman spectra of nGL films supported on a SiO2:Si substrate and HOPG.
Fundamental Resonance of mechanical resonator under tenstion T
E is the Young’s modulus;
r is the mass density;
t, w, and L are the dimensions of the suspended graphene sheet;
and A is the clamping coefficient, 1.03 for doubly clamped beams
and 0.162 for cantilevers.
Fig. 2. (A) Amplitude versus frequency for a 15-nm-thick multilayer graphene resonator taken with optical drive. (Inset) An optical image of the resonator. Scale bar, 5 mm. (B) Amplitude versus frequency taken with optical drive for the fundamental mode of the single-layer graphene
resonator shown in Fig. 1B. A Lorentzian fit of the data is shown in red.
Fig. 3. (A) A plot showing the frequency of the fundamental mode of all the doubly clamped beams and cantilevers versus t/L2. Cantilevers, triangles; doubly clamped beams with t > 7 nm, filled squares; doubly clamped beams with t < 7 nm, open squares. All thicknesses are determined by AFM. The solid line is the theoretical prediction with no tension and E = 1 TPa. The dashed lines correspond to E = 0.5 TPa and 2 TPa. (B) The quality factor of the fundamental mode versus thickness for all resonators measured.
Fig. 4. (A) Noise power density versus frequency taken at a resolution bandwidth of 1 kHz. (Inset) An optical image of the resonator. The resonator has dimensions t=5nm, L=2.7 mm, and w=630 nm. Scale bar, 2 mm. (B) Amplitude of resonance and quality factor versus dVg for Vgdc=2V.
The ultimate limit on the force sensitivity is set by the thermal fluctuations in the resonator:
The force sensitivity for the graphene resonator is observed to be 0.9 fN/Hz½.
The corresponding charge sensitivity dQf = dFfd/Vgdc = 8 × 10−4 e/Hz½,
where d is the distance between the graphene sheet and the gate electrodes.
FIG. 1. a A SEM micrograph of a graphene sheet suspended above a trench horizontal stripe etched in silicon dioxide. The sheet measured 7 nm thick by AFM. b An optical micrograph of a different suspended few-layer
graphene sheet measured to be 2 nm thick by AFM.
FIG. 2. A schematic of an AFM tip that is deflected while pushing down on
a suspended graphene sheet. graphene is measured by the AFM and hgrapheneis calculated using Eq. 4.
FIG. 3. (a) On the left axis is the curve obtained by the AFM while pushing down on a suspended graphene sheet. The right axis is the corresponding force. (b) Graph of force vs displacement of the suspended sheet. The spring
constant of the sheet is the slope of these data.
FIG. 4. (a) A surface plot of the spring constant of a suspended graphene sheet vs the location of the AFM tip. (b) An amplitude AFM micrograph of the suspended sheet measured to obtain (a) and imaged in by SEM in Fig. 1a. Each data point was taken at the intersection of the grid located on the suspended portion of the graphene. The trench etched into the silicon dioxide is seen as a vertical stripe.
FIG. 5. A plot of the spring constant as measured in the center of the suspended
region of the graphene sheets, vs wt /L3 for eight different samples. From the linear fit, we are able to extract an average tension and a Young’s modulus. The dashed line is the fit to all the data points, whereas the solid line is the fit for 7/8 of the data.